# Rietveld refinement

Rietveld refinement

Rietveld refinement is a technique devised by Hugo Rietveld for use in the characterisation of
crystalline materials. The neutron and x-ray diffraction of powder samples results in a pattern characterised by peaks in intensity at certain positions. The height, width and position of these peaks can be used to determine many aspects of the materials structure.

The Rietveld method uses a least squares approach to refine a theoretical line profile until it matches the measured profile. The introduction of this technique was a significant step forward in the diffraction analysis of powder samples as, unlike other techniques at that time, it was able to deal reliably with strongly overlapping reflections.

The method was first reported for the diffraction of monochromatic neutrons where the peak position is reported in terms of the Bragg angle 2"&theta;". This terminology will be used here although the technique is equally applicable to alternative scales such as x-ray energy or neutron time-of-flight. The only wavelength and technique independent scale is in reciprocal space units or momentum transfer "Q", which is historically rarely used in powder diffraction but very common in all other diffraction and optics techniques. The relation is

$Q = frac \left\{4 pi sin left \left( heta ight \right)\right\}\left\{lambda\right\}$

Peak shape

The shape of a powder diffraction peak is influenced by the characteristics of the beam, the experimental arrangement, and the sample size and shape. In the case of monochromatic neutron sources the convolution of the various effects has been found to result in a peak almost exactly Gaussian in shape. If this distribution is assumed then the contribution of a given peak to the profile yi at position 2"&theta;"i is:

$y_i = I_k exp left \left[ -4 ln left \left( frac\left\{2\right\}\left\{H_k^2\right\} ight \right) left \left(2 heta_i - 2 heta_k ight \right)^2 ight \right]$

where "H"k is the full width at half peak height (full-width half-maximum), 2"&theta;"k is the centreof the peak, and Ik is the calculated intensity of the peak (determined from the structure factor, the Lorentz factor, and multiplicity of the reflection)

At very low diffraction angles the peaks may acquire an asymmetry due to the vertical divergence of the beam. Rietveld used a semi-empirical correction factor, As to account for this asymmetry

$A_s = 1 - left \left[ frac \left\{sP left \left(2 heta_i - 2 heta_k ight \right)^2\right\}\left\{tan heta_k\right\} ight \right]$

where P is the asymmetry factor and s is +1,0,-1 depending on the difference 2&theta;i-2&theta;kbeing positive, zero or negative respectively.

At a given position more than one diffraction peak may contribute to the profile. The intensity is simply the sum of all peaks contributing at the point 2&theta;i.

Peak width

The width of the diffraction peaks are found to broaden at higher Bragg angles. This angular dependency was originallyrepresented by

$H_k^2 = U an^2 heta_k + V an heta_k + W$

where U, V and W are the halfwidth parameters and may be refined during the fit.

Preferred orientation

In powder samples there is a tendency for plate- or rod-like crystallites to align themselves along the axis of a cylindrical sample holder. In solid polycrystalline samples the production of the material may result in greater volume fraction of certain crystal orientations (commonly referred to as texture). In such cases the peak intensities will vary from that predicted for a completely random distribution. Rietveld allowed for moderate cases of the former by introducing a correction factor:

$I_\left\{corr\right\} = I_\left\{obs\right\} exp left \left(-Galpha^2 ight \right)$

where Iobs is the intensity expected for a random sample, G is the preferred orientation parameter and α is the acute angle between the scattering vector and the normal of the crystallites.

Refinement

The principle of the Rietveld Method is to minimise a function M which represents the difference between a calculated profile y(calc) and the observed data y(obs). Rietveld defined such an equation as:

$M = sum_\left\{i\right\} W_i left \left\{ y_i^\left\{obs\right\} - frac\left\{1\right\}\left\{c\right\} y_i^\left\{calc\right\} ight \right\}^2$

where Wi is the statistical weight and c is an overall scale factor such that $y^\left\{calc\right\} = c y^\left\{obs\right\}$

References

*cite journal
author=H. M. Rietveld
year=1969
title=A profile refinement method for nuclear and magnetic structures
journal=Journal of Applied Crystallography
volume=2
pages=65–71
doi=10.1107/S0021889869006558

*http://www.ccp14.ac.uk/ccp/web-mirrors/hugorietveld/xtal/paper2/paper2.html

* [http://home.planet.nl/~rietv025/ The Rietveld Method] - the story.
* [http://www.ing.unitn.it/~maud/ The MAUD program] - software for Rietveld refinement.

Wikimedia Foundation. 2010.

### Look at other dictionaries:

• Rietveld — Rietveld, Dutch for field of reed , can refer to:* Rietveld refinement (Crystallography), a powerful computational method for extracting detailed crystal structure information from X ray and neutron powder diffraction data. Named after Hugo M.… …   Wikipedia

• Hugo Rietveld — Hugo M. Rietveld is a Dutch crystallographer and one of the most prominent crystallographers of the 20th century. He is famous for his invention of the Rietveld refinement method, which is used for the characterisation of crystalline materials… …   Wikipedia

• Methode de Rietveld — Méthode de Rietveld Pour les articles homonymes, voir Rietveld. La méthode de Rietveld est une méthode d analyse en diffractométrie de rayons X sur poudre. Elle fut développée en 1969 par le cristallographe néerlandais Hugo Rietveld. Cette… …   Wikipédia en Français

• Méthode De Rietveld — Pour les articles homonymes, voir Rietveld. La méthode de Rietveld est une méthode d analyse en diffractométrie de rayons X sur poudre. Elle fut développée en 1969 par le cristallographe néerlandais Hugo Rietveld. Cette méthode consiste à simuler …   Wikipédia en Français

• Méthode de rietveld — Pour les articles homonymes, voir Rietveld. La méthode de Rietveld est une méthode d analyse en diffractométrie de rayons X sur poudre. Elle fut développée en 1969 par le cristallographe néerlandais Hugo Rietveld. Cette méthode consiste à simuler …   Wikipédia en Français

• Méthode de Rietveld — Pour les articles homonymes, voir Rietveld. La méthode de Rietveld est une méthode d analyse en diffractométrie de rayons X et de neutrons sur poudre. Elle fut développée en 1969 par le cristallographe néerlandais Hugo Rietveld. Cette méthode… …   Wikipédia en Français

• Neutron diffraction — Science with Neutrons Foundations Neutron temperature Flux · Radiation  …   Wikipedia

• X-ray scattering techniques — are a family of non destructive analytical techniques which reveal information about the crystallographic structure, chemical composition, and physical properties of materials and thin films. These techniques are based on observing the scattered… …   Wikipedia

• Maud — Not to be confused with Maude. As a feminine given name: Main article: Maud (name) As a placename: In Antarctica: Queen Maud Land (Norwegian: Dronning Maud Land), an area of 2.5 million square kilometers claimed by Norway in 1938 In Canada: Queen …   Wikipedia

• Western architecture — Introduction       history of Western architecture from prehistoric Mediterranean cultures to the present.       The history of Western architecture is marked by a series of new solutions to structural problems. During the period from the… …   Universalium